#------------------------------------------------------------------------------
#$Date: 2021-11-06 07:22:36 +0200 (Sat, 06 Nov 2021) $
#$Revision: 270340 $
#$URL: file:///home/coder/svn-repositories/cod/cif/1/56/51/1565134.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1565134
loop_
_publ_author_name
'Meyer, N.A.'
'Wenz, M.D.'
'Walsh, J.P.S.'
'Jacobsen, S.D.'
'Locock, A.J.'
'Harris, J.W.'
_publ_section_title
;
 Goldschmidtite, (K,REE,Sr)(Nb,Cr)O3: A new perovskite supergroup mineral
 found in diamond from Koffefontein, South Africa
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1345
_journal_page_last               1350
_journal_paper_doi               10.2138/am-2019-6937
_journal_volume                  104
_journal_year                    2019
_chemical_formula_sum
'Al0.01 Ba0.09 Ce0.08 Cr0.19 Fe0.05 K0.5 La0.15 Mg0.04 Nb0.7 O3 Sr0.13 Ti0.01'
_chemical_name_common
(K0.50La0.15Sr0.13Ba0.09Ce0.08)(Nb0.70Cr0.19Fe0.05Al0.01Mg0.04Ti0.01)O3
_chemical_name_mineral           goldschmidtite
_space_group_IT_number           221
_space_group_name_Hall           '-P 4 2 3'
_space_group_name_H-M_alt        'P m -3 m'
_cell_angle_alpha                90.000000
_cell_angle_beta                 90.000000
_cell_angle_gamma                90.000000
_cell_formula_units_Z            1
_cell_length_a                   3.98760(10)
_cell_length_b                   3.98760(10)
_cell_length_c                   3.98760(10)
_cell_volume                     63.407(3)
_diffrn_ambient_pressure         100
_diffrn_ambient_temperature      298
_cod_data_source_file            goldschmidtite.cif
_cod_data_source_block           goldschmidtite
_cod_original_cell_volume        63.404(6)
_cod_original_formula_sum
'K0.50 La0.15 Sr0.13 Ba0.09 Ce0.08 Nb0.70 Cr0.19 Fe0.05 Al0.01 Mg0.04 Ti0.01 O3'
_cod_database_code               1565134
loop_
_space_group_symop_id
_space_group_symop_operation_xyz
1 x,y,z
2 -x,-y,-z
3 -x,-y,z
4 x,y,-z
5 -x,y,-z
6 x,-y,z
7 x,-y,-z
8 -x,y,z
9 z,x,y
10 -z,-x,-y
11 z,-x,-y
12 -z,x,y
13 -z,-x,y
14 z,x,-y
15 -z,x,-y
16 z,-x,y
17 y,z,x
18 -y,-z,-x
19 -y,z,-x
20 y,-z,x
21 y,-z,-x
22 -y,z,x
23 -y,-z,x
24 y,z,-x
25 y,x,-z
26 -y,-x,z
27 -y,-x,-z
28 y,x,z
29 y,-x,z
30 -y,x,-z
31 -y,x,z
32 y,-x,-z
33 x,z,-y
34 -x,-z,y
35 -x,z,y
36 x,-z,-y
37 -x,-z,-y
38 x,z,y
39 x,-z,y
40 -x,z,-y
41 z,y,-x
42 -z,-y,x
43 z,-y,x
44 -z,y,-x
45 -z,y,x
46 z,-y,-x
47 -z,-y,-x
48 z,y,x
loop_
_atom_site_label
_atom_site_occupancy
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_adp_type
_atom_site_B_iso_or_equiv
_atom_site_type_symbol
KA 0.5040 0.500000 0.500000 0.500000 Uani 0.0111(12) K
LaA 0.1498 0.500000 0.500000 0.500000 Uani 0.0111(12) La
SrA 0.1329 0.500000 0.500000 0.500000 Uani 0.0111(12) Sr
BaA 0.0922 0.500000 0.500000 0.500000 Uani 0.0111(12) Ba
CeA 0.0778 0.500000 0.500000 0.500000 Uani 0.0111(12) Ce
NbA 0.6950 0.000000 0.000000 0.000000 Uani 0.0090(13) Nb
CrB 0.1920 0.000000 0.000000 0.000000 Uani 0.0090(13) Cr
FeB 0.0509 0.000000 0.000000 0.000000 Uani 0.0090(13) Fe
MgB 0.0350 0.000000 0.000000 0.000000 Uani 0.0090(13) Mg
AlB 0.0139 0.000000 0.000000 0.000000 Uani 0.0090(13) Al
TiB 0.0110 0.000000 0.000000 0.000000 Uani 0.0090(13) Ti
O 1.0 0.000000 0.500000 0.000000 Uani 0.012(2) O
